6. Single molecule analysis of DNA nanotube polymerization
6.2.4. Data acquisition
Since polymerization is temperature sensitive, we paid close attention to the temperature of our sample and minimized exposure to the room temperature.
Before the injection of DNA monomers, the empty sample chamber was mounted onto the heated prism and under the heated objective and immersion water to bring the sample chamber to the desired steady state temperature. Skipping this step will result in a sample chamber that is initially at room temperature, which would cause DNA nanotubes to nucleate very rapidly. In addition, our autofocus did not work well when the temperature of the sample, prism, and objective changed rapidly, such as in the initial heating step of our method of temperature control. The chamber was left empty at the desired steady state reaction temperature until the polymerization mix was ready.
In contrast to adding a liquid sample to a filled chamber, injecting a sample into an empty capillary chamber results in a known initial sample concentration. Previously, studies that used a similar sample chamber would flush the filled chamber with at least twice the chamber volume to ensure that the reaction conditions held during measurements. Because the fluid flow approaches zero near the channel walls, it is difficult to produce samples with known concentration using that method. The second advantage of starting with an empty chamber is fast injection time. Due to stronger capillary action, injecting the sample into an empty chamber requires less time than infusing a filled chamber with sample. The fast injection may also be important in minimizing thermal contact between the heated liquid of DNA tiles, DNA nanotubes, and the ambient room temperature.
However, an empty chamber also possesses an intrinsic problem; the fast injection flow of DNA nanotubes, especially at high temperatures, induces DNA nanotube scission. We minimized the scission problem by adding the sample gently at the opening of the empty chamber. The injection time was approximately 5 sec for.6µL sample. Quantifying how much scission occurs with our injection protocol is not necessary since the polymerization rate measurements should be independent of the initial amount of fragmentation.
We identified three instances in our protocol in which the polymerization mix was ex- posed to ambient environment. First, we pipetted 5µL methylcellulose to a supersaturated tile solution with a pipette tip that was at room temperature. Second, after we incubated the solution of supersaturated tiles and methylcellulose at 50 ◦C, we took the sample out from the temperature cycler and mixed it for ≈ 5 sec at room temperature. Third, we injected the supersaturated tiles, methylcellulose, and pre-formed DNA nuclei at the opening of the heated glass capillary chamber with a pipette tip that was not heated. To minimize the potential problem, such as the rapid nucleation of DNA nanotubes from supersaturated DNA tiles before the sample was injected to the heated glass capillary chamber, we performed these three steps as rapidly as we could. The typical execution time for these steps was 5 sec and no longer than 10 sec. In almost all cases, the fast sample handling seems to be sufficient to avoid spontaneous nucleation before imaging, with the exception of a polymerization assay at 600 nM and 41.4 ◦C. An extrapolation of the polymerization model predicted a net negative polymerization rate at600 nM and 41.4 ◦C (see the bottom right plot of Fig. 6.5). While the model may be true in an ideal protocol, we consistently observed spontaneous nucleation in our 600 nM and 41.4◦C movie. We attribute the observed nuclei as a result of spontaneous nucleation that was triggered by the brief exposure to room temperature during one or more of the steps discussed in this section.
DNA nanotube imaging
Our prism-based TIRF microscope, equipped with temperature control and automated fo- cusing, monitored the dynamics of the DNA nanotubes that were confined close to the glass surface (Figs.6.3and6.4) for more than 2 hours of imaging. The signal to noise ratio was very high, even in the presence of a high concentration of Cy3-labeled free monomers in solution. For all of the nanotubes that were analyzed, we did not encounter any pausing of polymerization in any of our movies, which provides evidence that the untreated glass surface is not too sticky. The majority of DNA tiles were in the free monomer state. The typical total concentration of DNA tiles in pre-formed DNA nuclei was less than
10 nM, which is 10×smaller than the most dilute free monomer concentration in our assay (100 nM). Even after 2 hours of imaging, we typically observed a difference of less than a factor of 2 in contour length for all DNA nanotubes, which corresponded to a small DNA tile concentration change.
In the reaction conditions where spontaneous nucleation was hardly observable, the DNA nanotube polymerization was followed for at least 1 hour and no longer than 2 hours. Much to our surprise, our imaging protocol did not require an oxygen scavenger buffer to achieve and maintain a high signal-to-noise ratio for more than 2 hours of time-lapse imaging. At an acquisition rate of typically 4 frames/min, we usually acquired enough data points in less than 30 minutes. If significant spontaneous nucleation was observed, we terminated the data acquisition after∼5 minutes because the newly formed nuclei rapidly obscured the visibility of the pre-formed nuclei. Moreover, the new nuclei can also end-to-end join to a growing DNA nanotube end, which made our polymerization rate measurements unreliable. Thus, spontaneous nucleation limited the range of temperatures and concentrations for which we could obtain accurate rate measurements.